3.2 Source and Drain
3.2.3 Aluminum Deposition and Diffusion
In order to have an estimation of the deposition rates of aluminum (and silicon oxide), the following process was tested in the clean room:
• deposition through sputtering of 20nm of SiO2;
• measurement of deposited SiO2 film thickness through an ellipsometer;
• deposition through sputtering of 100nm of Al;
• photoresist (PR) deposition, exposure, development;
• measurement through a profilometer of PR with respect to Al;
• Al etching, and measurement through profilometer of PR with respect to SiO2. Regarding the deposition process, it was realized with the Sputter AJA (AJA In-ternational Inc.) shown in Fig.3.19 giving as results the data provided in Tab.3.4.
Figure 3.19: Sputter AJA used for testing the aluminum deposition rate in the clean room.
Table 3.4: Process parameters for aluminum and silicon oxide deposition.
Target Thickness Pressure Power Ar Flow Dep. Rate Time
SiO2 20nm 4mtorr 100W 10sccm 0.11 30min
Al 100nm 4.1mtorr 80W 10sccm 0.2 1.38h
The deposition rates (provided by the machine itself) are quite low, thus suggesting an overall minimum deposition process time of about two hours. After the silicon oxide deposition, three measurements with an ellipsometer were taken giving as results the data collected in Tab.3.5, while an example of the ellipsometer output is given in Fig.3.20.
Figure 3.20: Third ellipsometer measurement for the silicon oxide thickness.
The measurement results are consistent with the inputs provided to the sputtering machine: the oxide thickness is around 20nm.
Table 3.5: Ellipsometer measurement data for the silicon oxide thickness.
Measurement 1 20.974nm± 0.17.7nm Measurement 2 20.970nm± 0.17.6nm Measurement 3 20.947nm± 0.16.6nm
After the silicon oxide thickness measurement, aluminum was deposited (Tab.3.4) and the following procedure was followed for the photoresist deposition:
• wafer cleaned with Isopropanol;
• bake 2min at 115°C;
• spin coating, through Spinner 2 AB Plast Spin 150, of positive PR s1813:
– time: 30s.
– speed: 3000RP M.
• bake 1min at 115°C.
and then were exposed through a Mask Aligner EVG 620, where the used mask was composed of arrays of squares, giving as result the structure in Fig.3.21.
Figure 3.21: Wafer used for testing the deposition process after exposure.
Then the exposed photoresist was developed with MF 3189, and through a Pro-filometer DEKTAK 150, three measurements in a row in the middle of the wafer were carried out giving as results the data collected in Tab.3.6.
Table 3.6: Profilometer measurement data for the estimation of the photoresist thickness in three different squares.
Measurement 1 1009.60nm Measurement 2 1005.08nm Measurement 3 1003.32nm
Therefore approximately a 1µm thick PR layer was deposited. Then the aluminum was etched with Aluminium Etch 16:1:1:2, and the structure in Fig.3.22 was ob-tained.
Figure 3.22: Wafer used for testing the deposition process after aluminum etching.
The dark areas are made of silicon oxide.
Then three measurements (along the same squares in of Tab.3.6) with the profilome-ter were taken, providing the data in Tab.3.7.
Table 3.7: Profilometer measurement data for the estimation of the aluminum thick-ness in three different squares.
Measurement 1 1122.40nm Measurement 2 1120.10nm Measurement 3 1120.16nm
It is important to remark that every measurement is done in the same associated square (that is Measurement 1 in Tab.3.6 is taken on the same square on which then Measurement 1 in Tab.3.7 is carried out) in order to have a coherent result. Sub-tracting the measurements in Tab.3.6 from the ones in Tab.3.7, gives an estimation of the deposited aluminum thickness (Tab.3.8):
Table 3.8: Profilometer measurement data for the aluminum thickness.
Al thickness 1 112.80nm Al thickness 2 115.02nm Al thickness 3 116.84nm
The thickness of the deposited aluminum layer is larger than the expected one (110nm), but this is not considered critical for the fabrication process, since the aluminum is going to be used as metallization material.
Once the aluminum is deposited, a diffusion process is necessary in order to make it diffuse in the silicon, thus lowering the semiconductor resistivity. The process can be modelled as a constant dose diffusion process, that is the concentration is assumed to have a gaussian distribution :
N (x, t) = Q0
• Q0 (atoms/cm3) is the deposited dose;
• D = D0e−(EakT) (cm2/s) is the diffusion coefficient;
• D0 (cm2/s) is an extrapolated constant;
• Ea (eV ) is the activation energy;
• k (eV/K) is the Boltzmann constant;
• T (K) is the temperature;
• t (s) is the time.
The critical point is to understand how to set the time t and temperature T in order to obtain a quasi constant distribution in the p++ regions, and how to estimate the
deposited dose Q0. The latter is a complex parameter, since its value is dependent on the crystalline structure of the deposited material, and the deposition technique.
But a simple estimation can be done in the following way:
Q0 = N0ρAlTAl
• N0 (mol−1)is the number of Avogadro;
• ρAl (kg/cm3) is the aluminum density;
• TAl (cm) is the thickness of the deposited layer;
• mAl (g/mol) is the aluminum molar mass.
That is, multiplying the density by the thickness of the deposited layer the surface density is obtained. So dividing the latter by the molar mass the number of moles square centimeter is obtained. Multiplying the latter by the Avogadro number pro-vides the number of atoms per square centimer. Regarding the choice of the time and the temperature, they are critically important since the dependence in Eq.3.10 is exponential. Thus a MATLAB code was implemented (Appendix A.5) to under-stand the influence of these parameters on the estimated diffusion process; a fixed temperature of 1300K (which is the maximum achievable temperature in the facil-ity) was assumed, and the concentration profile was computed for different diffusion times, giving as results the plots in Fig.3.23.
Figure 3.23: Concentration profile assuming a temperature of 1300K and a pre-deposited layer of 20nm for different diffusion times.
As expected, by increasing the time, the concentration is lowering at the surface, and the profile is less steep . If instead of an aluminum deposited layer of 20nm, a thickness of 200nm is considered, the concentration profile presents higher dopants at the surface (Fig.3.24). This makes sense since in the expression provided for the dose estimation (Eq.3.11), the latter is obtained by multiplying the area density by the deposited layer thickness, so it is assumed that thicker is the deposited layer, and higher is the constant dose at the surface.
Figure 3.24: Concentration profile assuming a temperature of 1300K and a pre-deposited layer of 200nm for different diffusion times.
Since a high doping concentration implies a reduction of the parasitic resistance, a deposition of 200nm of aluminum is considered. Regarding the diffusion, a 3h process at 1300K guarantees, at least ideally, a more flat profile.
It is important to remark that the presented analysis is not considering fabrica-tion process effects such as lateral diffusion, and diffusion caused by the deposifabrica-tion temperature during the layer deposition step. Thus it represents a theoretical esti-mation.